Carbon Fibre Reinforced Polymer Composites
with Enhanced Ductility
A dissertation submitted in partial fulfilment of the requirements for the degree of Doctor of Philosophy of Imperial College London
Department of Chemical Engineering Imperial College London South Kensington Campus,
Carbon fibre reinforced polymers (CFRPs) have high strength and stiffness, low density, long fatigue life in the fibre direction and good corrosion resistance. Nowadays, CFRPs are been used in aeronautics, wind turbine blades, sports goods and civil industry. However, one fundamental limitation of CFRPs is their brittleness (low ductility): CFRPs fail catastrophically at a relatively low strain (1.5% to 1.8%) under the tension with little warning or residual load-carrying capacity. To overcome this weakness, there is considerable interest to enhance the ductility of CFRPs exhibiting increased failure strains under tension and more progressive, graceful failure modes.
In this work, three different methods were developed to improve the ductility of unidirectional (UD) CFRPs. The first method was to introduce fibre waviness into UD composites. The fibre alignment angles of the resulting composites and control composites were assessed and it was found that fibre waviness in UD composite did result in a stepwise tensile failure mode and an enhanced strain to failure. The second method was using an air-assisted fibre tow spreading and commingling technology to manufacture continuous intermingled carbon fibre/glass fibre hybrid tows. After defining and quantifying the degree of hybridisation (at the filament level) of two carbon fibre/glass fibre hybrid tows, the one with the higher degree of hybridisation was selected to manufacture intermingled UD hybrid composites. It was found that hybridising of continuous glass and carbon fibres resulted in the composites with an increased failure strain. Moreover, these hybrid composites failed more gradually. The final method investigated for introducing ductility was the introduction of ply cuts into PEEK interleaved UD carbon fibre/PEEK composites, which were manufactured by compression moulding. The resulting cut-ply interleaved carbon
fibre/PEEK composite possessed a non-linear tensile stress-strain curve and ductility strain of 0.4%, which is due to shearing of the PEEK interleaves in the overlap regions between the cut carbon fibre plies.
Declaration of Originality
This dissertation is a description of the work carried out by the author in Department of Chemical Engineering, Imperial College London between October 2010 and November 2014 under the supervision of Prof. Alexander Bismarck and Prof. Paul Robinson. Except where acknowledged, the material presented is the original work of the author and no part of it has been submitted for a degree at this or any other university.
The copyright of this thesis rests with the author and is made available under a Creative Commons Attribution Non-Commercial No Derivatives licence. Researchers are free to copy, distribute or transmit the thesis on the condition that they attribute it, that they do not use it for commercial purposes and that they do not alter, transform or build upon it. For any reuse or redistribution, researchers must make clear to others the licence terms of this work.
First of all, I would like to thank my PhD supervisors, Profs Alexander Bismarck and Paul Robinson from Imperial College London and Prof. Michael Wisnom from the University of Bristol for their patient guidance, consistent encouragement and helpful discussions during the past four years. They have been sharing their extensive knowledge, great passion and valuable expertise in composite materials, which inspired me and also improved my work skills for the future.
I would like to express my gratitude to UK Engineering and Physical Sciences Research Council (EPSRC) for providing financial support to part of my research via Programme Grant EP/I02946X/1 on High Performance Ductile Composite Technology (HiperDuCT).
I am grateful to Dr. John Hodgkinson for valuable and prompt modification of my PhD thesis manuscript, helpful suggestions about mechanical testing methods for composite materials and expert advice on the characterisation of fibre misalignment angles. I am indebted to Dr. Soraia Pimenta for her modelling skills in predicting tensile behaviour of hybrid carbon/glass fibre composites and cut-ply interleaved carbon fibre/PEEK composites. I would like to thank Gary Senior, Jonathan Cole and Mark Grant for their help on composite manufacturing and sample preparation, Joseph Meggyesi for his patient tuition on mechanical testing of composite materials, Dr. Jesper Ankersen and Dr. Carla Gispert for their assistance with DIC measurements.
I would like to express my gratitude to all the members in Polymer and Composite Engineering (PaCE) group, who were always helpful and provided joy not only in research but also in daily life. I would like to thank (not in any particular order) Dr. Kingsley Ho, Dr. Siti Rosminah Shamsuddin, Dr. Koon Yang Lee, Dr. Sheema Riaz,
Dr. Henry Maple, Dr. Robert Woodward, Dr. Derrick Fam, Dr. Hui Qian, Dr. Atif Javaid, Dr. Natasha Shirshova, Su Bai, Dr. Edyta Lam, Jing Li, Michael Tebboth, Francois De Luca, Dr. Tomi Herceg, Wan Wan Nawawi, Dr. Jonny Blaker, Dr. Min Tang, Dr. Andreas Mautner, Dr. Ling Ching Wong, Dr. Qixiang Jiang and Dr. Nadine Graeber. Also, I would like to thank all the supervisors (Prof. Michael Wisnom, Prof. Ian Bond, Dr. Sameer Rahatekar, Prof. Kevin Potter, Prof. Paul Weaver, Prof. Alexander Bismarck, Prof. Paul Robinson, Prof. Milo Shaffer, Dr. Pimenta Soraia, Prof. Paul Curtis and Dr. Silvestre Pinho) and researchers (Dr. Omar Bacarreza Nogales, Dr. David Anthony, Francois De Luca, Dr. Gael Grail, Dr. Gergely Czel, Dr. HaNa Yu, Dr. James Serginson, James Trevarthen, Jonathan Fuller, Dr. Meisam Jalalvand, Dr. Siti Rosminah Shamsuddin and Stefano Del Rosso) involved in HiperDuCT project, a true collaboration between Imperial College and the University of Bristol, for their helpful discussions and advice during the monthly meetings. Last, but not the least, I am deeply grateful to my parents, Riming Diao and Hongwen He. They nurtured my interest in science and engineering when I was a child and encouraged and supported me to study overseas when I grew up. During all those years, they gave me their deepest and endless love. Without them, I would not have finished my PhD successfully. Thanks for everything you did for me!
Table of contentsAbstract ... 2 Declaration of Originality ... 4 Copyright Declaration ... 5 Acknowledgement ... 6 Table of contents ... 8 List of figures ... 13 List of tables ... 19 List of abbreviation ... 21 1 Introduction ... 22
1.1 Aims and objectives ... 23
1.2 Structure of thesis ... 25
2 Indication of the potential of making UD CFRPs with the enhanced tensile strain via introducing fibre waviness ... 26
2.1 Introduction ... 26
2.2 Literature review ... 27
2.2.1 The effect of fibre waviness and misalignment on the tensile behaviour of UD composites ... 27
2.2.2 Manufacturing techniques to produce composites containing wavy fibres….………30
2.2.3 Methodology of measuring fibre waviness and fibre misalignment ... 33
2.3.1 Materials ... 36
2.3.2 Manufacturing UD carbon fibre/PA-12 with fibre waviness ... 36
2.3.3 Single-fibre tensile tests on as-received and gas-textured carbon fibres41 2.3.4 Tensile tests of control, gas-textured and non-constrained annealed carbon fibre/PA-12 tapes ... 43
2.3.5 Measuring fibre alignment angle in carbon fibre/PA-12 composites .... 44
2.4 Results and discussion ... 46
2.4.1 Effect of gas-texturing on the tensile properties of carbon fibres ... 46
2.4.2 Tensile behaviour of control, gas-textured and non-constrained annealed carbon fibre/PA-12 tapes ... 47
2.4.3 The fibre alignment angle in the control, gas-textured and non-constrained annealed carbon fibre/PA-12 tapes ... 50
2.5 Summary ... 53
3 Intermingled carbon fibre/glass fibre thermosetting hybrid composites ... 55
3.1 Introduction ... 55
3.2 Literature review ... 57
3.2.1 The definition and classification of fibre hybrid composites... 57
3.2.2 Tensile behaviour of UD fibre hybrid composites ... 58
3.2.3 Manufacturing of UD fibre hybrid composites ... 66
3.3 Materials and methods ... 69
3.3.1 Materials ... 69
3.3.3 Microscopy analysis of carbon fibre/glass fibre hybrid tows ... 74
3.3.4 Determination of fibre diameters ... 75
3.3.5 Manufacturing of carbon fibre/glass fibre reinforced epoxy hybrid composite ... 76
3.3.6 Tensile test of carbon fibre/glass fibre reinforced epoxy composite ... 77
3.4 Results and discussion ... 78
3.4.1 Spreading and comingling of carbon fibre/glass fibre tows ... 78
3.4.2 Characterisation of the degree of the hybridisation of carbon fibre/glass fibre tows ... 86
3.4.3 Degree of hybridisation of carbon fibre/glass fibre hybrid fibre tows ... 97
3.4.4 Tensile properties of carbon fibre/glass fibre reinforced epoxy composites... 99
3.5 Summary ... 101
4 Ductile cut-ply interleaved carbon fibre/PEEK composites ... 103
4.1 Introduction ... 103
4.2 Literature review ... 105
4.3 Materials and method ... 106
4.3.1 Materials ... 106
4.3.2 Cut-ply interleaved carbon fibre/PEEK design ... 107
4.3.3 Manufacturing method of cut-ply interleaved carbon fibre/PEEK ... 109
4.3.4 Tensile test method of cut-ply interleaved carbon fibre/PEEK ... 113
4.4 Results and discussion ... 116
4.4.1 The micro-structure of cut-ply interleaved carbon fibre/PEEK composite ………..116
4.4.2 Tensile behaviour of cut-ply interleaved carbon fibre/PEEK composite ………..120
4.4.3 Fractographic analysis of the cut-ply interleaved carbon fibre/PEEK composite ... 124
4.5 Summary ... 124
5 Conclusions and future work ... 126
5.1 Summary of findings ... 126
5.1.1 Introducing fibre waviness into UD composites ... 126
5.1.2 Intermingled UD carbon fibre/glass fibre hybrid composites ... 127
5.1.3 Interleaved cut-ply carbon fibre/PEEK composites ... 128
5.1.4 Comparison of the three approaches to produce CFRP with enhanced ductility ………..128
5.2 Suggestions for future work ... 130
5.2.1 Introducing fibre waviness into UD composites ... 130
5.2.2 Intermingled UD carbon fibre/glass fibre hybrid composites ... 131
5.2.3 Interleaved cut-ply carbon fibre/PEEK composite ... 132
Appendix I ... 134
Appendix II ... 137
List of figures
Figure 2.1 Predicted and experimental tensile stress-strain curves of (±θ)S carbon fibre/PEEK composite  ... 27 Figure 2.2 (a) Schematic drawing of representative volume and coordinates for UD composite with uniform fibre waviness, (b) photo showing UD composite with uniform fibre waviness and (c) predicted and experimentally obtained tensile stress-strain curves for UD composite with uniform fibre waviness but various fibre waviness ratios  ... 29 Figure 2.3 Schematic diagrams of manufacturing techniques to produce thermosetting composites containing ply waviness (a) , (b) [32, 33, 35], (c) and (d) [35, 36] .... 31 Figure 2.4 Schematic drawing of a sinusoidal-model waved fibre  ... 33 Figure 2.5 Unidirectional carbon/epoxy composite with out-of-plane ply waviness ... 34 Figure 2.6 (a) Optical micrograph of UD composite with a domain and pixel array highlighted and (b) schematic depiction of a set of domains within which the average ... 35 Figure 2.7 (a) Photo and (b) flow chart of setup of manufacturing route of UD carbon fibre/PA-12 composite tape ... 36 Figure 2.8 Design of gas-texturing device (a) photo (b) schematic diagram ... 37 Figure 2.9 Setup of (a) 13 pins used in wet-impregnation bath and (b) 3 heated shear pins ... 38 Figure 2.10 Schematic diagram of layup process of carbon fibre/PA-12 tapes during non-constrained annealing ... 39 Figure 2.11 Mould temperature during the non-constrained annealing process ... 40
Figure 2.12 Top views of the carbon fibre/PA-12 tape (a) before and (b) after
non-constrained annealing ... 40
Figure 2.13 Mounting for single fibre tensile test specimen (a) Dimensions of mounting (b) Mounting with specimen bonded in place ... 42
Figure 2.14 Setup of single-fibre tensile test ... 42
Figure 2.15 The dimensions of the tensile specimen ... 43
Figure 2.16 Setup for tensile tests of UD composite tapes ... 43
Figure 2.17 (a) Schematic diagram of cutting sample (b) Typical microscopy image of polished sample surface ... 44
Figure 2.18 Distribution of the apparent fibre alignment angles of a typical gas-textured carbon fibre/PA-12 sample ... 45
Figure 2.19 Typical tensile stress-strain plots of as-received and gas-textured carbon fibres ... 46
Figure 2.20 (a) The cumulative failure curve and (b) Weibull plots of as-received and gas-textured carbon fibres ... 47
Figure 2.21 Tensile stress-strain curves of (a) control, (b) gas-textured and (c) non-constrained annealed carbon fibre/PA-12 tapes ... 50
Figure 2.22 True fibre alignment angle distributions of (a) control (b) gas-textured and (c) non-constrained annealed carbon fibre/PA-12 composites ... 51
Figure 3.1 Classification of fibre hybrid composites: (a) laminated, (b) woven and (c) intermingled ... 58
Figure 3.2 Theoretical tensile strength of fibre hybrid composite  ... 66
Figure 3.3 Schematic figure of air-assisted fibre spreading process  ... 70
Figure 3.4 Setup of fibre tow spreading machine (a) photo (b) flow chart ... 71
Figure 3.6 Manufacturing of intermingled carbon fibre /glass fibre tow ... 74 Figure 3.7 Typical micrograph of a carbon fibre/glass fibre hybrid tow (type B) ... 75 Figure 3.8 (a) Schematic diagram and (b) photo of the setup used to measure fibre diameters using the modified-Wilhelmy technique ... 76 Figure 3.9 (a) Schematic and (b) photo of the mould used to manufacture carbon fibre/glass fibre reinforced epoxy hybrid composite ... 77 Figure 3.10 Dimensions of the specimen used for the tensile testing ... 77 Figure 3.11 Photos of carbon fibre and glass fibre tows taken during fibre spreading 83 Figure 3.12 Appearance of same spread carbon fibre (CF-H) tow with and without twists ... 84 Figure 3.13 Appearance of carbon fibre/glass fibre hybrid tows (a) Type A and (b) Type B ... 85 Figure 3.14 Schematic diagrams of ideal intermingled fibre hybrid tow containing two fibre types in the (a) hexagonal fibre package and (b) cubic fibre package ... 87 Figure 3.15 Schematic of the model to describe randomly-distributed, comingled two fibre-type hybrid tow ... 87 Figure 3.16 Probability distribution of APCF,Model for a model fibre hybrid tow type B when the model was run 1, 10, 100 and 1000 times at the sizes of analysis windows of (a) 3x3 (b) 6x6, and (c) 14x14 fibres ... 89 Figure 3.17 Coefficient of variation in APCF,Model for fibre hybrid tow type B at as function of the size of the analysis window and number of times the model was run 90 Figure 3.18 Flow chart of the program to evaluate the distribution of carbon fibre and glass fibre in micrographs of cross-sections of carbon fibre/glass fibre hybrid tows .. 91
Figure 3.19 Detection of carbon fibres and glass fibres from original micrograph using an image recognition program: (a) original micrograph, (b) carbon fibre within the micrograph and (c) glass fibre within the micrograph ... 92 Figure 3.20 Schematic of subdividing the micrograph into square analysis windows 93 Figure 3.21 Probability distributions of APCF,Model and APCF,Experiment for fibre hybrid tow type B as function of the size of analysis windows (a) (3Dnominal)2, (b) (6Dnominal)2and (c) (14Dnominal)2 ... 96 Figure 3.22 Coefficients of variation in APCF,Model and APCF,Experiment as a function of
size ... 97 Figure 3.23 Characteristic optical micrographs of cross-sections of fibre hybrid tow A (a and b) and fibre hybrid tow B (c and d) ... 99 Figure 3.24 Typical tensile stress-strain curves of control carbon fibre/epoxy, carbon fibre/glass fibre/epoxy and control glass fibre/epoxy (Vf =30-40%, VCF:VGF = 1.55:1) ... 100 Figure 4.1 Schematic diagram of cut-ply interleaved carbon fibre/PEEK composite ... 104 Figure 4.2 Schematic diagrams of UD discontinuous tow composite laminates  ... 106 Figure 4.3 Analysis of the unit cell in the cut-ply interleaved carbon fibre/PEEK composite ... 108 Figure 4.4 Photo of the mould for manufacturing small-scale interleaved carbon fibre/PEEK composite ... 110 Figure 4.5 (a) Schematic diagram and (b) photo of the mould for manufacturing large-scale cut-ply interleaved carbon fibre/PEEK composite ... 112 Figure 4.6 Schematic diagrams of cutting template (a) A and (b) B ... 113
Figure 4.7 (a) Schematic diagram from the side view and (b) photo of the tensile test setup ... 114 Figure 4.8 Definition of initial modulus, y,y, εu and
d ... 115 Figure 4.9 Schematic diagram of fracture surface of cut-ply interleaved carbon fibre/PEEK ... 115 Figure 4.10 The thicknesses of PEEK region in small-scale interleaved carbon fibre/PEEK composites manufactured from the PEEK films with the thicknesses of (a) 100 μm and (b) 50 μm via various temperature and pressure used in compression moulding ... 117 Figure 4.11 The micrographs of small-scale interleaved carbon fibre/PEEK composites made from (a) 50-μm-thick PEEK film (sample: S-8)and (b) 100-μm-thick PEEK film (sample :S-4) ... 118 Figure 4.12 The micro-structure of the large-scale cut-ply interleaved carbon fibre/PEEK composites obtained using cutting templates (a) A and (b) B ... 119 Figure 4.13 The schematic diagram of micro-structural changes in cut-ply interleaved carbon fibre/PEEK composite caused by compression moulding ... 120 Figure 4.14 The typical tensile stress-strain curves measured from the front and back view at the gauge length of 10 mm ... 121 Figure 4.15 The micrographs of a cut-ply interleaved carbon fibre/PEEK composite observed from the (a) front and (b) back views ... 122 Figure 4.16 A typical plot of the effect of the gauge length on the strain to failure and modulus of the cut-ply interleaved carbon fibre/PEEK composite ... 123 Figure 4.17 The typical tensile stress-strain curves of cut-ply interleaved carbon fibre/PEEK composite at the gauge length of 6,8 10 and 12mm ... 123
Figure 4.18 The SEM images of PEEK fracture surface of cut-ply interleaved carbon fibre/PEEK composite at the magnifications of (a) 1000 x and (b) 1600 x ... 124 Figure 5.1 Schematic diagram of interleaved cut-ply carbon fibre/PEEK composite containing multiple overlapping regions ... 133
List of tables
Table 2.1 Operation parameters of polishing process ... 44 Table 2.2 Tensile properties of as-received and gas-textured carbon fibre ... 47 Table 2.3 Tensile properties of control, gas-textured and non-constrained annealed carbon fibre/PA-12 composite tapes ... 48 Table 2.4 Parameters of the Gaussian fitting curves of the distribution of the fibre alignment angles of control, gas-textured, non-constrained annealed carbon fibre/PA-12 composite ... 52 Table 3.1 Overview of the investigations on the hybrid effect of continuous UD fibre hybrid composites ... 61 Table 3.2 Comparisons of ultimate failure strain of the hybrid composites and their corresponding un-hybridised composites ... 65 Table 3.3 The detail information of carbon fibres ... 69 Table 3.4 The detail information of glass fibres ... 70 Table 3.5 Summary of function, component and operating parameters of fibre tow spreading machine ... 71 Table 3.6 The manufacturing parameters of spreading carbon fibre and glass fibre tows ... 72 Table 3.7 Fibre types, number of filaments of each fibre type and volume ratio between carbon fibre and glass fibre in the carbon fibre/glass fibre hybrid tows ... 73 Table 3.8 The manufacturing parameters of hybridising carbon fibre/glass fibre tows ... 74 Table 3.9 Grading system used to quantify stability of the spread fibre tow width .... 79 Table 3.10 Summary of the appearance of spread carbon fibre and glass fibre tows .. 80 Table 3.11 Diameters of the fibres used in hybridisation ... 88
Table 3.12 Tensile strength, modulus, strain to initial and final failure of control CF/epoxy, CF/GF/epoxy and control GF/epoxy composites. ... 101 Table 4.1 Properties of carbon fibre/PEEK prepreg and PEEK [7, 118] ... 107 Table 4.2 Manufacturing parameters of compression moulding of small-scale interleaved carbon fibre/PEEK composite ... 110 Table 4.3 The micro-structure of cut-ply interleaved carbon fibre/PEEK (produced by cutting templates and measured in the micrographs) ... 120 Table 4.4 The tensile properties of cut-ply interleaved carbon fibre/PEEK composite ... 120 Table 5.1 The tensile properties of the composites produced using wavy fibres, hybrid tows and by ply cutting and interleaving ... 129
List of abbreviation
CF Carbon fibre
CFRP Carbon fibre reinforced polymer CPL Composite production line CV Coefficient of variation
CTE Coefficient of thermal expansion
DIC Digital image correlation
FE Finite element
FRP Fibre reinforced polymer
GF Glass fibre
GFRP Glass fibre reinforced polymer HDPE High density polyethylene
NDE Non-destructive evaluation
PEEK Polyether ether ketone
ROM Rule of mixtures
SEM Scanning electron microscopy
Conventional fibre reinforced polymer composites (FRPs) possess high strength and stiffness, low density, long fatigue life in fibre direction and an excellent resistance to corrosion. By carefully selecting the type and amount of reinforcement, its alignment and orientation in a polymer matrix, these composites offer a wide range of mechanical properties, which hence provide immense design possibilities. Within the last fifty years the production of fibre reinforced polymer composites has rapidly increased. It is estimated that the global consumption of carbon fibre reinforced polymers (CFRPs) will reach $25.2 billion by 2020  and the market for glass fibre reinforced polymers (GFRPs) will be worth $16.4 billion in 2016 . In the early days, the application of carbon fibre reinforced polymer composites was mainly confined to the aeronautics industry . In the recent decades, CFRPs have become widely used in other areas such as wind turbine blades, pressure vessels, luxury automobiles, civil construction, marine applications and a vast variety of sports goods. Despite the advantages of high performance CFRPs, such as their high specific strength and stiffness, these materials have a fundamental limitation, which is their inherent brittleness. Conventional UD CFRPs deform elastically to the strain of ~1.5% [4-7] and then fail catastrophically with no prior warning or little residual load-carrying capacity. In contrast, some ductile materials, such as some metals and polymers, can deform plastically with much higher strains to failure and hence dissipate significant strain energy. The terminology “ductility” is initially used to describe the ability of solid material to deform plastically under tension without fracture [9-11]. However, this definition is not quite suitable to describe the ductility of UD CFRPs, because the tensile properties of UD CFRPs in fibre direction are dominated by carbon fibre, which has no ductility. In this thesis, the definition of
ductility for UD CFRPs is mainly referred to whether the CFRPs have an improved failure strain under tension with a progressive and graceful failure mode.
Due to the lack of ductility of conventional CFRPs, the CFRPs have very limited residual load carrying capacity after the initial failure occurs. To overcome this limitation, it is necessary to increase the ductility of CFRPs and this could be achieved by creating composites with enhanced strain to failure and a more progressive failure mode. However, to-date much of the research focussed on improving FRP composite materials has been directed towards improving their through-thickness properties, i.e. improving delamination resistance and impact performance, and, more recently, the development of multifunctional [12-15] and green FRPs [16-20]. Despite achieving plastic deformation of CFRPs using angle-ply composites [21-23], it seems that little work has been directed towards improving the ductility of CFRPs. Much more work was published related to enhancing the ductility of CFRPs used in construction materials [24-26]. However, even in civil engineering, there has only been a very limited work done for this purpose. In Bank’s review paper  about ductility of FRP composites for civil construction, he stated that “there has been insufficient attention to exploiting and enhancing progressive failure and energy absorption in the FRP composites themselves”. It is therefore necessary to develop methods to enhance the ductility of FRP exhibiting increased failure strains and more progressive, graceful failure modes.
1.1 Aims and objectives
In 2011, Imperial College London and University of Bristol launched a six-year research programme, i.e. high performance ductile composite technology (HiperDuCT), to design, realise and evaluate composite architectures that display a
ductile or pseudo-ductile response to mechanical load while maintaining high strength and stiffness.
As part of HiperDuCT programme, the research stated in this thesis is aimed to develop CFRP composites with enhanced ductility, which exhibit increased failure strains and a more progressive failure mode. Three different approaches (corresponding to three technical chapters in the thesis) have been explored to achieve this objective. The three approaches include introducing fibre waviness into UD composite (Chapter 2), mixing carbon and glass fibres at the filament level to create ideally intimately intermingled UD hybrid composites (Chapter 3) and adding polymer interleaves into cut-ply UD composites (Chapter 4).The specific objectives are listed below:
a) Chapter 2
Create UD CFRP with randomly distributed wavy fibres
Characterise the fibre alignment angles and tensile properties of such composites
b) Chapter 3
Manufacture continuous UD intermingled carbon/glass fibre hybrid composites and characterise their tensile behaviour
Define and quantify the degree of hybridisation (at filament level) in such composites
c) Chapter 4
Produce a cut-ply interleaved carbon fibre/PEEK composite and characterise its tensile behaviour
1.2 Structure of thesis
The thesis is divided into five chapters. Chapter 1 provides a general introduction and defines the aims and objective of this research. Chapter 2, 3 and 4 describe the three approaches taken to develop CFRPs with enhanced ductility. Each of these three chapters includes an introduction, an individual literature review, descriptions of the manufacturing techniques, test methods and test results, a discussion and a summary of the key findings. The final chapter of this thesis provides an overall summary and conclusion of this research as well as the suggestions for future work.
Indication of the potential of making UD CFRPs with the
enhanced tensile strain via introducing fibre waviness
Unidirectional (UD) carbon fibre reinforced polymers (CFRPs) have high specific strength and stiffness, but they fail in a brittle manner with little warning when subjected to uniaxial tension. This inherent brittleness means that the material has no load-carrying capacity after the initial failure occurs. Changing the failure mode of UD CFRPs from catastrophic one into gradual one and improving the failure strain of UD CFRPs, therefore, could potentially reduce the required safety factors. The tensile properties of UD CFRPs in the fibre direction are dominated by the fibre properties. It has already been demonstrated that the waviness and fibre misalignment can enhance the tensile failure strain and produce a non-linear tensile behaviour [22, 23, 27-30], and this will be discussed in section 2.2. One of the possible failure mechanisms of a composite containing fibres with various waviness and misalignment is that straight and well-aligned fibres fail first while the tensile load can stretch and align the wavy, misaligned fibres in direction of the applied strain until they eventually fail. However, most work described in previous literature [22, 23, 27-30] focused on theoretical prediction of the tensile behaviour of UD composite with uniform fibre waviness. There is little published work available on the experimental tensile behaviour of UD composites with small fibre misalignment angle and random fibre waviness.
In this chapter, the literature about the effect of fibre misalignment and fibre waviness on the tensile behaviour of CFRPs, the manufacturing techniques and characterisation of fibre misalignment and fibre waviness in CFRPs, are reviewed first. Inspired by the possibility of tailoring the tensile strain to failure and producing a non-linear failure behaviour, two manufacturing methods were explored for producing UD composites
containing wavy fibres with small degrees of fibre misalignment. Gas-texturing the carbon fibre tow and non-constrained annealing carbon fibre/PA-12 were used to produce such UD composites. The fibre alignment angles and tensile properties of these two composites and their control samples were characterised.
2.2 Literature review
2.2.1 The effect of fibre waviness and misalignment on the tensile behaviour of UD composites
Before investigating the effect of fibre or ply misalignment and waviness on the tensile behaviour of UD composite, researchers firstly began to study the tensile behaviour of angle-ply (±θ)S composites to evaluate the effect of fibre alignment angle on the tensile behaviour of composites [22, 23, 27, 28]. As can be seen in Figure 2.1 , the tensile stress- strain behaviour of UD angle-ply (±θ)S composites exhibits a significant non-linearity. Even though larger fibre alignment angles result in a significant reduction of the tensile strength and modulus compared with UD composites, introducing (±θ)S fibre alignment angles does provide composites with non-linear tensile stress-strain curves and a more progressive failure behaviour.
Figure 2.1 Predicted and experimental tensile stress-strain curves of (±θ)S carbon fibre/PEEK composite 
Compared with (±θ)S angle-ply composite, the tensile behaviour of UD composites with ply waviness is more complex, because composites with ply waviness contain different fibre alignment angles within a single ply. Chou and Takahashi  predicted using an elastic constitutive model that Kevlar or glass fibre reinforced elastomers containing uniform out-of-plane ply waviness exhibit a non-linear tensile behaviour and enhanced tensile failure strain. Later, Chun et al.  built a model to investigate the tensile behaviour of UD carbon fibre/epoxy composites with uniform out-of-plane fibre waviness and validated the model experimentally, as shown in Figure 2.2 (a) and (b). They found that the apparent modulus of such composite was reduced as the tensile stress increased. The non-linear tensile behaviour and the failure strain increased with increasing fibre waviness , as shown in Figure 2.2 (c). Unfortunately, both models showed that introducing uniform fibre waviness reduced the tensile strength and modulus compared with the UD composites.
Figure 2.2 (a) Schematic drawing of representative volume and coordinates for UD composite with uniform fibre waviness, (b) photo showing UD composite with uniform fibre waviness and (c) predicted and experimentally obtained tensile stress-strain curves for UD composite with uniform fibre waviness but various fibre waviness ratios 
In order to minimise the reduction in the tensile strength and modulus caused by introducing uniform fibre waviness into the UD composites and to produce composites with an enhanced failure strain exhibiting a non-linear tensile behaviour, it is desirable to design UD composite containing wavy and straight fibres, In such a
composite, the straight fibres will fail first but the undamaged wavy fibres can still carry the load. Such composite, therefore, would fail in steps rather than in a catastrophic manner.
2.2.2 Manufacturing techniques to produce composites containing wavy fibres
18.104.22.168 Producing thermosetting composites containing wavy fibres
In the 1990s, researchers began to develop processes to introduce fibre waviness or ply waviness into carbon fibre/epoxy composites. Kuo et al.  manufactured an out-of-plane wavy UD carbon fibre/epoxy composite by using a sinusoidal matching mould, shown in Figure 2.3(a). Later, some investigators added carbon fibre/epoxy strip into UD composite when laying up UD prepregs to create a UD carbon fibre/epoxy with out-of-plane ply waviness, as seen in Figure 2.3 (b) [32, 33]. Potter et al.  reported that fibre misalignment and in-plane waviness in uncured UD carbon fibre/epoxy prepregs (maximum fibre misalignment angle of 3.8°) is mainly caused by the variation in tension applied on the carbon fibres tows when manufacturing UD prepregs, the twisting within fibre tows, the presence of broken fibres, which lay across the fibre direction of the prepreg and winding the prepreg for the storage and delivery. Later, they also produced out-of-plane wavy-ply carbon fibre/epoxy composites by a carefully designed moulding process. They added a carbon fibre/epoxy strip (Figure 2.3(b)), one or two UD discontinuous carbon fibre/epoxy layers (Figure 2.3(c) and (d)) into a number of continuous UD carbon fibre/epoxy prepregs during the layup process to form a composite with controlled out-of-plane ply waviness . They found that the presence of ply-waviness can cause delamination initiating at the ply drops, which negatively affected the compressive strength of the UD composites .
Figure 2.3 Schematic diagrams of manufacturing techniques to produce thermosetting composites containing ply waviness (a) , (b) [32, 33, 35], (c) and (d) [35, 36]
22.214.171.124 Producing thermoplastic composites containing wavy fibres
UD carbon fibre/thermoplastic composites with out-of-plane ply waviness were reported by Mrse and Piggott, who designed a crimping moulding method to introduce ply waviness into carbon fibre/PEEK composites . The authors found that this process damaged the carbon fibres, which had a negative effect on the compressive strength of the composite . O’Hare and Hyer  developed a three-step moulding method to manufacture flat cross-wavy ply carbon fibre/polysulfone (PSU) composites. This moulding method involved creating the wavy ply using a curved matched mould, then using strips made of carbon fibre/PSU to fill the gaps between the curved layer and the nearby flat layers to form a flat sub-laminate, finally laying up the sub-laminate with other carbon fibre/PSU layers and consolidating them into laminate .
As stated above, using curved moulds can only introduce waviness into UD carbon fibre/thermoplastic composite at ply level, some published work shows that some continuous UD fibre reinforced thermoplastic composites manufactured by fibre commingling by gas-texturing can contain a degree of waviness at fibre level [39-42]. In the 1990s, fibre gas-texturing technology was developed to comminglereinforcing
Carbon fibre/epoxy (fibre in x direction) Carbon fibre/epoxy (fibre in y direction)
z x y
fibre yarns and thermoplastic polymer fibre yarns to form a hybrid roving, which was then processed into continuous fibre reinforced thermoplastic polymers using pultrusion process . Lauke et al.  reported that the longitudinal tensile strength of UD glass fibre reinforced polyamide produced by consolidation of glass fibre/polyamide fibre hybrid tows was lower than the value predicted by the rule of mixture but they did not provide tensile stress-strain curves of this composite. The authors thought that the reduction in tensile strength was caused by the fibre misalignment in the composite, because some fibre misalignment was observed in the fibre hybrid tow. However, it seems likely that the damage on the glass fibres caused by gas-texturing process is another factor contributing to the reduction of tensile strength of such composite.
Thermal expansion, on the other hand, can produce waviness at filament level without damaging the fibre. Some investigations show the coefficient of thermal expansion (CTE) mismatch between the composite materials and mould tools , CTE mismatch between fibre and thermoplastic matrix  can cause the residual thermal stress in fibres, which is large enough to create fibre waviness in UD composite. Kugler and Moon observed a fibre waviness with a maximum degree of fibre misalignment of 8.4° in a carbon fibre/PSU composite when investigating the effect of different processing parameters (mould materials, moulding temperature and time) on fibre waviness in the resulting composites . The heating/cooling history during processing of fibre reinforced thermoplastics can affect the magnitude of the fibre waviness or misalignment in the composite . Cohen et al.  observed fibre waviness in a single glass fibre reinforced polycarbonate sample, which was caused by polymer melt flow during the consolidation process.
2.2.3 Methodology of measuring fibre waviness and fibre misalignment
The magnitude of fibre waviness affects the mechanical behaviour of UD composites. One of the major problems in characterising fibre waviness is the need to determine or define the shape of a wavy fibre. Many researchers assumed a sinusoidal form (Figure 2.4) when modelling wavy fibres [30, 46-48]. The magnitude of the ideal fibre waviness can be quantified by the wavelength (λ) and the amplitude (A) of a sinusoidal wavy fibre. The maximum fibre misalignment angle is a function of wavelength and amplitude (Equation 2.1):
Figure 2.4 Schematic drawing of a sinusoidal-model waved fibre 
However, the problem is that most wavy fibres are in reality not sinusoidal, which makes it difficult to determine fibre misalignment angles using Equation 2.1. Most researchers, therefore, measured the ply or fibre misalignment angle directly to quantify ply or fibre waviness. The out-of-plane ply misalignment can be easily observed and measured from micrographs of cross-section of the composite in through-thickness direction [35, 38, 48], as seen in Figure 2.5. Recently, Pain and Drinkwater  also developed a non-destructive evaluation method to detect and locate the ply waviness using ultrasonic array scattering. In this method, the average
) 2 ( tan 1 max A 0.0 0.5 1.0 1.5 2.0 -2 -1 0 1 2 max Y() y= Asin(2*x/) X() A Nominal fibre direction
ultrasonic array scattering matrix of a UD composite without ply waviness was generated from experimental ultrasonic scanning and statistics-based signal processing, which was treated as a baseline; the ply waviness in a UD composite was detected and located by comparing the signals obtained from experimental ultrasonic scan on this wavy composite with the baseline.
Figure 2.5 Unidirectional carbon/epoxy composite with out-of-plane ply waviness However, measuring fibre misalignment angles of individual fibres is more challenging than measuring the ply waviness, because it requires a detection technique with higher resolution. Since the 1980s, several researchers have investigated the characterisation of fibre misalignment from the micrographs of polished section of composites [50-54]. Two of the most popular methods for measuring fibre misalignment are Yurgartis’ method  and multi-field image analysis [52, 54]. Yurgartis used the fact that a fibre with a circular cross section will be an ellipse when cut at an angle other than 90° and 0° to the fibre direction. By measuring the major and minor axial dimensions of the ellipsoid, the individual fibre alignment angle can be obtained. The accuracy of this method was reported to be ± 0.25º . This method will be discussed in detail in section 2.2.3. Creighton and Sutcliffe [52, 54] designed a multi-field image analysis to determine the degree of fibre misalignment in a composite from a low magnification microscope image. In their method, the fibre alignment angle in a domain (250 x 250 μm) of a longitudinal
section of a UD composite was inferred from the alignment of the elongated features, which can be a fibre filament, fibre bundle or the matrix between the fibres, as shown in Figure 2.6. This method is less time-consuming and more effective in measuring the fibre misalignment in a large domain than Yurgartis’ method, but the results obtained were less reliable when the domain size was decreased [52, 54].
Figure 2.6 (a) Optical micrograph of UD composite with a domain and pixel array highlighted and (b) schematic depiction of a set of domains within which the average fibre orientation φ is to be measured 
2.3 Materials and methods
Continuous carbon fibre tows (HexTow®IM7-12K) kindly provided by Hexcel Co. (Cambridge, UK) were used as reinforcement. Polyamide (PA)-12 in powder form (Vestosint®-2159, Evonik Degussa GmbH, Weiterstadt, Germany) was used as matrix. Nitrogen (BOC UK Co. London, UK) was used in the gas-texturing process. 2.3.2 Manufacturing UD carbon fibre/PA-12 with fibre waviness
126.96.36.199 Manufacturing unidirectional carbon fibre/PA-12 composite tapes using
gas-texturing method followed by wet-powder impregnation
Gas-textured carbon fibre/PA-12 tape was manufactured using a modular custom-built composite production line (CPL)  (developed by Polymer and Composite Engineering Group in Imperial College London), shown in Figure 2.7.
Figure 2.7 (a) Photo and (b) flow chart of setup of manufacturing route of UD carbon fibre/PA-12 composite tape
A 2 L PA-12 suspension (5 wt.%) was prepared for the wet-impregnation bath in the CPL. In order to aid the dispersion of the polymer powder and avoid cake formation during rest periods, 0.1 wt.% surfactant (Cremophor® A-25, BASF Company, Manchester, UK) was added to the suspension. In order to ensure that PA-12 powder
Melt oven Heated shear pins Tension control Gas-texturing
device Polymer suspension Dry oven Two-belt puller Fibre
was homogenously distributed in the impregnation bath, this suspension was stirred for 2.5 h. Similarly, 1L concentrated PA-12 suspension (15 wt%) was prepared as the top-up material to maintain the polymer concentration in the wet-impregnation bath during the manufacture process as otherwise the dispersion would deplete.
Two carbon fibre tows were passed over a perforated PTFE bar (Figure 2.8). A N2 (pressure=2.5 bar) flow passing through these small holes (Øhole = 1 mm) in the bar caused the carbon fibre tows to spread into filaments or small bundles and some fibre misalignment. These spread carbon fibre tows were combined into one carbon fibre tow after the gas-texturing process.
Figure 2.8 Design of gas-texturing device (a) photo (b) schematic diagram
The tow was then passed through the PA-12 wet-impregnation bath alternating under and over 13 pins (Figure 2.9(a)) to increase the space between the filaments in the tow to allow them to pick up PA-12 powder from the suspension. Two 1 m long infra-red heating ovens were used to remove the water carried by the fibre tow (set temperature: 120°C) and melt the polymer powder (set temperature: 205°C), respectively. The fibre tow with the polymer melt passed over and under three heated shear pins (set temperature: 220°C; Figure 2.9(b)), which provided the composite tape with a smooth surface. Finally, it was consolidated between the two room-temperature steel rollers. A two-belt puller was used to control the speed of this manufacturing process at 0.5 m/min. 20 mm Øhole = 1 mm Øbar =16 mm N2 N2 1mm (b) (a)
Figure 2.9 Setup of (a) 13 pins used in wet-impregnation bath and (b) 3 heated shear pins
Control carbon fibre/PA-12 composite tapes were manufactured using the same method as the gas-textured carbon fibre/PA-12 except that the fibre tow did not pass over the gas-texturing device. During this process, the concentration of polymer powder in the wet-impregnation bath decreases, which results in an increasing fibre volume fraction in the composite. In order to maintain the powder concentration 50 mL concentrated PA-12 suspension (15 wt.%) was, therefore, added into the bath every 15 min. The fibre volume fraction of the composite (Vf), calculated using Equation 2.2, was monitored by weighing 1 m of the composite tape:
Equation 2.2 where ρ is the density of the materials (g/m3), W the linear weight of the tape (g/m). The subscripts c, m and f represent composite, polymer matrix and fibre, respectively. Only composite tapes with Vf = 58-62% were selected in this research.
188.8.131.52 Manufacturing of carbon fibre/PA-12 composite tape using
In order to introduce fibre misalignment into carbon fibre/PA-12 without damaging carbon fibres, the composite tapes were annealed at temperature from 220 °C to 20 °C when non-constrained. In this process, two factors cause carbon fibre misaligned after moulding: a) PA-12 remains a viscous melt for a sufficient long time allowing the carbon fibres to move as the melt flows; b) the CTE mismatch between carbon fibres
f m f c f f m f W W W W V ) ( (a) (b)
and PA-12 and the CTE mismatch between composite and mould causes residual thermal stress in carbon fibres, which in turn cause the carbon fibres to become misaligned and wavy during the consolidation.
Figure 2.10 Schematic diagram of layup process of carbon fibre/PA-12 tapes during non-constrained annealing
The carbon fibre/PA-12 tape with a width of 6-8 mm was cut into 200 mm long sections. These tape sections were sandwiched between release films (Upilex® 25S, UBE Industries Ltd., Tokyo, Japan) and placed between two steel plates, as seen in Figure 2.10. The whole assembly was heated in a pre-heated hot press (Model# 4126, Carver Inc., Indiana, USA) at 220°C with contact-only pressure (i.e. no actual pressure applied) for 2 h. It was slowly cooled down to room temperature in 8 hours. The temperature change of the unit was monitored by a thermocouple (RS 615-8206, RS Components Co., UK), which is shown in Figure 2.11. After the non-constrained annealing, some visible fibre misalignment was introduced into the carbon fibre/PA-12 tape, as seen in Figure 2.fibre/PA-12. However, the magnitude of the fibre misalignment angle cannot be clearly quantified from Figure 2.12 due to the low magnification of the images.
Mould release film CF/PA-12
Figure 2.11 Mould temperature during the non-constrained annealing process
Figure 2.12 Top views of the carbon fibre/PA-12 tape (a) before and (b) after non-constrained annealing -50 0 50 100 150 200 250 300 350 400 450 500 550 600 20 40 60 80 100 120 140 160 180 200 220 240 T emp era tu re ( o C) Time (min) (a) (b) 1 mm 1 mm
2.3.3 Single-fibre tensile tests on as-received and gas-textured carbon fibres A Linkam TST350 tensile tester (Linkam Scientific Instrument Ltd, Surrey, UK) with 20N load cell was used to measure the tensile strength and the apparent modulus of as-received and gas-textured carbon fibre according to the ISO 11566 standard . Single fibres were mounted onto paper cards (seen in Figure 2.13) to minimize the stress concentration on the fibre in the gripping area. A single fibre was placed at the centre of the testing card and bonded at both ends of the mounting using an epoxy adhesive (Araldite® Rapid, Huntsman Advanced Materials GmbH, Switzerland). The fibre specimen on the paper mount was fixed in the grips, shown in Figure 2.14. Then, both sides of the cardboard holder were cut at the mid gauge. The single fibres were loaded at a crosshead rate of 15 μm/s. The load-crosshead displacement curve was recorded until the fibre failed. 25 single fibres from each group, i.e. as-received and gas-textured, were tested in order to obtain a representative result. The tensile strength ( ) and strain to failure ( ) of the fibres were calculated using Equation 2.3 and Equation 2.4, respectively.
Equation 2.3 Equation 2.4 where Fmax is the maximum measured tensile load, d the fibre diameter, δ the crosshead displacement when the fibre fails and L the gauge length. The apparent tensile modulus E is the slope of the linear fit to the tensile stress-strain curve.
ˆ2 max 4 ˆ d F L ˆ
Figure 2.13 Mounting for single fibre tensile test specimen (a) Dimensions of mounting (b) Mounting with specimen bonded in place
Figure 2.14 Setup of single-fibre tensile test
In order to evaluate the variation and distribution of the carbon fibre tensile strength, the cumulative failure probability PR,i of the ith fibre was calculated using Equation 2.5. The Weibull-modulus (m) of the fibre strength is given by the slope of
PR,i as function of ln plot, see Equation 2.6 ,
Equation 2.5 Equation 2.6 where Ri is the rank of the ith fibre, N the total number of tested fibres, the strength of the ith fibre and C a constant.
ˆ1 , N R P i i R C m PRi i ln(1 )] lnˆ ln[ , i
ˆ(a) (b) Enlarge Load cell Grips Paper mounted specimen
2.3.4 Tensile tests of control, gas-textured and non-constrained annealed carbon fibre/PA-12 tapes
All the carbon fibre/PA-12 tapes were cut into 200 mm-long sections and end tabbed with glass fibre/epoxy laminate with a thickness of 1.5 mm. The end tabs were bonded to the tape using cyanoacrylate adhesive (CN-general, Techni Measure Co, Japan). The dimensions of the tested samples are shown in Figure 2.15. The samples were tested under uniaxial tensile load (Model 4566 or 5969, Instron Ltd, Bucks, UK, depending on availability) at a crosshead rate of 0.5 mm/min. Digital image correlation (ARAMI-2M, GOM UK Ltd, Coventry, UK) was used to record the strain over the whole gauge length in the control and gas-textured carbon fibre/PA-12 samples. A video-gauge system (Imetrum Ltd, Bristol, UK) was used to measure the strain in the non-constrained annealed carbon fibre/PA-12. The setup for the tensile tests is shown in Figure 2.16.
Figure 2.15 The dimensions of the tensile specimen
Figure 2.16 Setup for tensile tests of UD composite tapes
Thickness (t) =0.08mm. Width (w) = 6-8mm Free length (L) =100mm Length of end tabs (e) =50mm
2.3.5 Measuring fibre alignment angle in carbon fibre/PA-12 composites
184.108.40.206 Microscopy sample preparation
After tensile testing, samples were cut from the undamaged end-tab regions at an angle of 5º nominal to the fibre direction (Figure 2.17(a)). The cut samples were embedded in a transparent epoxy resin (EpoCure®, Buehler Ltd., Düsseldorf, Germany) and cured at room temperature for 24 h. The samples were polished using a disc polish machine (Motopol-12, Buehler Ltd., Düsseldorf, Germany) with different grades of sand paper and diamond suspensions (details are given in Table 2.1). The polishing pressure and speed were 0.2 MPa and 150 rpm, respectively.
Table 2.1 Operation parameters of polishing process Polishing
sequence Polishing grade (min) Time
1 P120 SiC (with water as medium) 10
2 P320 SiC (with water as medium) 5
3 P800 SiC (with water as medium) 5
4 P2500 SiC (with water as medium) 5
5 Nylon cloth (with 6 μm diamond suspension as medium) 2 6 Nylon cloth (with 3 μm diamond suspension as medium) 2 7 Nylon cloth (with 1 μm diamond suspension as medium) 2
Figure 2.17 (a) Schematic diagram of cutting sample (b) Typical microscopy image of polished sample surface
220.127.116.11 Microscopy analysis
The cut surfaces of tested samples were investigated using a reflective microscope
(AX10, Zeiss Ltd., Cambridge, UK) at 50x magnification. Twenty microscopy images
were taken from each sample. A typical optical micrograph is shown in Figure 2.17(b). By measuring the major and minor axial dimensions of the cut fibre surfaces, the apparent fibre angle can be determined using Equation 2.7 :
Equation 2.7 where θapparent is apparent fibre alignment angle, l and d the major and minor axial dimensions of the cut fibre surfaces, respectively.
For each image, 10 fibres were randomly selected for measurement. Two hundred fibre alignment angles, therefore, were measured for each sample. As stated above, 4 samples in each group were tested in the uniaxial tensile test, so 800 apparent fibre alignment angles in each group (i.e. control, gas-textured and non-constrained annealed carbon fibre/PA-12) were characterised to obtain a representative result.
Figure 2.18 Distribution of the apparent fibre alignment angles of a typical gas-textured carbon fibre/PA-12 sample
The apparent fibre alignment angle θapparent is a function of the fibre alignment angle in the composite and the sectioning angle φs. However, the sectioning angle cannot be determined with a high accuracy by measuring the angle between the cut surface and fibre direction. Figure 2.18shows the distribution of apparent fibre alignment angle of a typical gas-textured carbon fibre/PA-12 tape. It is worth noting that only very few
l d apparent sin 1 0 1 2 3 4 5 6 7 8 9 10 11 12 0.0 0.1 0.2 0.3
Apparent fibre alignment anlge Gauss-fitting curve
Apparent fibre alignment angle ()
Vo lu me fra ct io n 2 2 ) ( 2 0 2 / ) ( w x x c e w A y x f Gauss fitting s=Xcentre=5.25 angle
fibres have an apparent fibre alignment angle smaller than 3°, which skews the apparent fibre alignment angle distribution. When the apparent fibre alignment is very small (less than 3°), the sectioned fibre segment shows as a quasi-rectangle, which has a length exceeding the length of microscopy measuring field. These fibre segments, therefore, were not countable in the measurement. In order to minimise the distortion caused by the limited microscopy measuring field, the sectioning angle is the median value (Xcentre) of the gauss-fitting curves of the apparent alignment angle distribution instead of the average value of the measured apparent fibre alignment angles. The true fibre alignment angle (θ) is determined via Equation 2.8.
2.4 Results and discussion
2.4.1 Effect of gas-texturing on the tensile properties of carbon fibres
The typical tensile stress-strain plots of as-received and gas-textured carbon fibre are shown in Figure 2.19. The tensile properties of as-received and gas-textured carbon fibre are shown in Table 2.2. The tensile strength and strain to failure of gas-textured carbon fibres is 15% lower than for as-received carbon fibres. As expected, the tensile modulus of the carbon fibres is hardly affected by the gas-texturing process.
0.0 0.5 1.0 1.5 2.0 0 1000 2000 3000 4000 5000 As-received Gas-textured St re ss (MPa ) Strain (%)
Figure 2.19 Typical tensile stress-strain plots of as-received and gas-textured carbon fibres
Table 2.2 Tensile properties of as-received and gas-textured carbon fibre Strength
(MPa) Strain to failure (%) Modulus (GPa) Weibull modulus of strength
As-received 4843 ±192 1.72±0.07 273.7±2.5 5.34
Gas-textured 4152± 201 1.48±0.08 267.4±4.2 4.37
The plots of tensile cumulative failure probability PR as function of the tensile strength σ of as-received and gas-textured carbon fibres fit well to the Weibull probability distribution (Figure 2.20). The Weibull modulus of as-received carbon fibres is 22% higher than that of gas-textured carbon fibres, which means that the scatter in the strength of the as-received fibres is lower.
Figure 2.20 (a) The cumulative failure curve and (b) Weibull plots of as-received and gas-textured carbon fibres
2.4.2 Tensile behaviour of control, gas-textured and non-constrained annealed carbon fibre/PA-12 tapes
The tensile strength, modulus and strain to failure of the control, gas-textured and non-constrained annealed carbon fibre/PA-12 tapes are summarised in Table 2.3. Because the tensile modulus of gtextured carbon fibre was same as that of as-received carbon fibre, the initial tensile modulus of gas-textured carbon fibre/PA-12 was barely changed compared to the control carbon fibre/PA-12 (165.9 GPa versus 164.9 GPa). Compared with the control carbon fibre/PA-12, the strength and the
0 2000 4000 6000 8000 10000 0.0 0.2 0.4 0.6 0.8 1.0 As-received Gas-textured
Boltzmann fit of as-received Boltzmann fit of gas-textured
C umu la tive fa ilu re p ro ba bi lit y P R Strength (MPa) 7.5 7.6 7.7 7.8 7.9 8.0 8.1 8.2 8.3 8.4 8.5 8.6 8.7 8.8 -4 -3 -2 -1 0 1 2 As-received Air-textured ln [-l n(1 -P R )] ln m=5.34 m=4.37 (b) (a) Gas-textured m=4.37 m=5.34
initial failure strain of carbon fibre/PA-12 composites manufactured using fibres which passed the gas texturing process decreased, which is because the carbon fibres were damaged during the gas-texturing process (see section 2.4.1). The gas flow does not only spread the fibres but also induced surface flaws or damage by fibre-fibre contact on the surface of the fibres, causing a reduction in strength and strain to failure of the carbon fibres. However, there was no reduction in tensile strength of the non-constrained annealed carbon fibre/PA-12 composite compared with the control samples, because the carbon fibres were protected by PA-12 melt during the non-constrained annealing process.
Table 2.3 Tensile properties of control, gas-textured and non-constrained annealed carbon fibre/PA-12 composite tapes
Modulus (GPa) Strength (MPa) Failure strain (%) Initial Ultimate
Control 165.9±9.7 2495±105 1.61±0.03
Gas-textured 164.9±7.4 2313±116 1.37±0.07 1.58±0.09 Non-constrained annealed 169.6±6.6 2491±158 1.51±0.08 1.96±0.16 It is interesting to note that the tensile stress-strain curves of the gas-textured and non-constrained annealed carbon fibre/PA-12 showed a stepwise, gradual failure mode during strain controlled tensile tests instead of the usual sudden, catastrophic failure, which was observed for the control carbon fibre/PA-12 samples (Figure 2.21). During the testing of the gas-textured and non-constrained annealed carbon fibre/PA-12 tapes, part of the sample still carried some load after the first failure occurred, while the control sample completely failed in a catastrophic manner. The difference in failure mode is associated with the difference in fibre alignment between the composites manufactured using carbon fibres that passed through the gas texturing process or which were subjected to the non-constrained annealing process and the control samples. The straight fibres will carry the greater stress and so are more likely to fail first. Of the remaining fibres those with least misalignment will fail next and so the
failure process was more gradual in the gas-textured and non-constrained annealed carbon fibre/PA-12 with their large spread of fibre alignment angles. However, due to the reduction in the tensile strength and failure strain of the fibres, which were subjected to the gas-texturing process, no increase was observed in the ultimate failure strain of gas-textured carbon fibre/PA-12 composites compared with the control samples. Nevertheless it is promising that a higher ultimate failure strain was observed for the carbon fibre/PA-12 composites which were subjected to non-constrained annealing compared to the control carbon fibre/PA-12. The higher ultimate failure strain for this composite was due to the fact that non-constrained annealing introduced significant fibre misalignment and waviness (see Figure 2.22) into the composite without damaging the carbon fibres. Compared with the control carbon fibre/PA-12 composite, the non-constrained annealed carbon fibre/PA-12 composite had enhanced ductility which exhibited in its higher ultimate failure strain and a more gradual failure mode.
Figure 2.21 Tensile stress-strain curves of (a) control, (b) gas-textured and (c) non-constrained annealed carbon fibre/PA-12 tapes
2.4.3 The fibre alignment angle in the control, gas-textured and non-constrained annealed carbon fibre/PA-12 tapes
In order to lend support for the proposed failure mechanism of the composites, containing the fibres which passed through the gas texturing process or were subjected to non-constrained annealing, the distributions of fibre alignment angles were quantified (Figure 2.22).
0 500 1000 1500 2000 2500 3000 0 500 1000 1500 2000 2500 3000 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6 1.8 2.0 2.2 0 500 1000 1500 2000 2500 3000 St re ss (MPa ) A B C D St re ss (MPa ) A B C D A B C D St re ss (MPa ) Strain (%) (a) (b) (c)
Figure 2.22 True fibre alignment angle distributions of (a) control (b) gas-textured and (c) non-constrained annealed carbon fibre/PA-12 composites
The true fibre alignment angles of the control, gas-textured and non-constrained annealed carbon fibre/PA-12 tapes ranged from -2 to 2°, -3.5 to 4° and -4 to 5°, respectively. It can be seen that the distribution are symmetric about the 0° degree position except for higher magnitude of misalignment in the gas-textured and non-constrained annealed composite. In these cases, there appears to be fewer fibres with misalignment angle less than -3°, then there are with angle greater than 3°. However, noted earlier, this is due to the difficulties with the measurement technique, fibres at angle close to -5° have major axis length which exceeded the length of the micrograph and so were not counted. Despite this loss of symmetry, the fibre
0.0 0.1 0.2 0.3 0.4 0.0 0.1 0.2 0.3 0.4 -10 -9 -8 -7 -6 -5 -4 -3 -2 -1 0 1 2 3 4 5 6 7 8 9 10 0.0 0.1 0.2 0.3 0.4 Vo lu me fra ct io n Control Gauss fitting Vo lu me fra ct io n Gas-textured Gauss fitting Vo lu me fra ct io n
Fibre alignment angle (, )
Non-constrained annealed Gauss fitting (b) (a) (c)
misalignment distributions of all these composites are fitted well by Gauss distribution. A Gaussian distribution as described is Equation 2.9:
Equation 2.9 where θc is the median value of the Gaussian fitting curve, y0 the offset value in y axis of the Gaussian fitting curve, A the area between the Gaussian fitting curve and y = y0 and w refer to the width of the peak in the Gaussian fitting curves. The width of the peak in the Gaussian fitting curves when is . Table 2.4 summarises the parameters of the Gaussian fitting curves of the fibre alignment angle distributions of the control, gas-textured, non-constrained carbon fibre/PA-12 composites. Compared with the control carbon fibre/PA-12, the widths of Gaussian fitting curves of the distributions of fibre alignment angles in the gas-textured and the non-constrained annealed carbon fibre/PA-12 increased by 77% and 116%, respectively. This indicates that both the annealing process and gas texturing significantly increase the variance of the fibre alignment angles in carbon fibre/PA-12 composites.
Table 2.4 Parameters of the Gaussian fitting curves of the distribution of the fibre alignment angles of control, gas-textured, non-constrained annealed carbon fibre/PA-12 composite θc (°) w A Control 0.00 1.00 0.49 Gas-textured 0.03 1.77 0.44 Non-constrained annealed 0.02 2.16 0.43
Ninety five percents of the fibres in the carbon fibre/PA-12 control had less than ±1° misalignment from the fully aligned position. However, only 68.5 % of fibres in the gas-textured carbon fibre/PA-12 composites were still almost straight, i.e. the misalignment angle smaller than ±1°. The bulk of the remaining 31.5 % were misaligned up to ±3°, but some fibres were misaligned to an even greater extend. This
2 2 ) ( 2 0 2 / ) ( w c e w A y f 2 / ) ( max 0 0 y y y y w ln4